3D Compression Molding


 Homer Hutchinson
 1 years ago
 Views:
Transcription
1 Autodesk Simulation Moldflow Insight D Compression Molding Executive summary In this work, the simulation results from a program developed for the threedimensional analysis of compression molding of thermoset composites are compared to the experimental results of an actual molded thermoset sample. The program predicts the flow pattern, fiber orientation, fiber length distribution, curing of the resin (for thermoset materials) and mechanical properties. The comparison between simulation and experiment includes short shots, fiber orientation and mechanical properties. Actual fiber orientation images were obtained using CT scanning. The comparison shows reasonable agreement between simulation and experiment.
2 Contents Introduction... 3 Governing Equations for Flow and Fiber Orientation Analyses... 4 Mechanical Properties Calculation... 5 An Example Case... 7 Conclusion Acknowledgements References
3 Introduction A compression molding process is illustrated in Figure 1. As can be seen from this figure, some portion of the cavity initially is filled by a charge (called initial charge ). The initial cavity thickness is much higher than the final part thickness. The mold cavity thickness is reduced by a compressive force, forcing the resin into the unfilled portions of the cavity. The compression by the press is generally done at a controlled speed until a maximum force is reached, but may sometimes be fully force controlled. After the cavity is filled, additional press movement may be required to compensate for polymer shrinkage. Figure 1: The schematic of the compression molding process. This compression molding process results in more homogeneous physical properties and less moldedin stresses compared to conventional injection molding. Also, for long fiber, compression molding has an advantage in that the final fiber length will have much less breakage than that obtained from injection molding due to attrition in injection unit and feed system. Long fiber composites processed by compression molding will retain most of their original fiber length leading to enhanced mechanical properties compared to short fiber composites. In this report, a threedimensional compression analysis program developed for thermoplastics and thermoset materials will be described. This program can predict the flow pattern, fiber orientation, fiber length distribution, curing (for thermoset materials) and mechanical properties. Fiber content, length and orientation greatly affect the performance of the product. The three dimensional analysis is chosen instead of a two dimensional analysis for the following reasons: Three dimensional analyses produce more accurate results for thick parts or parts with complicated geometry. The velocity and pressure in the compression direction can be calculated more accurately with three dimensional analyses. The initial charge geometry can be modeled more accurately. Designers and engineers can use the results from the program developed in this study to optimize the materials and process conditions. 3
4 In the next sections, an analysis method for the compression process for flow, fiber orientation and mechanical properties calculation will be given. This will be followed by some results from a case study. Governing Equations for Flow and Fiber Orientation Analyses We need to solve the following set of equations to analyze the flow during compression molding process for thermoplastics materials [1]: ( v) 0 t Dv p τ g Dt (1) (2) C p DT Dt 2 Dp ( kt ) T (3) Dt Equation (1) is the mass continuity equation, (2) the momentum equation and (3) the energy equation. For thermoset materials, equation (3) is modified to include a cure heating term as shown below: C p DT Dt 2 Dp D ( kt ) T H r (4) Dt Dt For thermoset materials, we also need to solve the curing kinetics equation. One example is the following Kamal s equation [2]: D Dt ( K1 K2 )(1 ) (5a) where K 1 E1 ( ( )) T 1 A e K 2 2 E2 ( ( )) T A e (5b) In the above equations, is density, t time, v velocity, p pressure, stress tensor, g gravitational constant of the earth. Also, C p is the heat capacity, T temperature, k thermal conductivity, viscosity, shear rate, expansivity and H r heat of 4
5 reaction. Furthermore, is degree of cure and A 1, A 2, E 1, E 2,, are constants used in the curing kinetics. A noslip boundary condition can be applied at the fixed noncompression mold wall as in regular injection molding analysis. However, unlike in regular injection molding, a specified speed boundary condition needs to be applied at the compression mold wall when the press is moving under speed control. When the press is moving under force control, the press speed needs to be calculated based on the press force. The fiber orientation is calculated for long fibers using the anisotropic rotary diffusion model combined with the reduced strain closure model (ARDRSC) as in [3]. da ( W A AW ) ( D A A D 2[ Α (1 )( L Μ : Α)]: D) dt (2[ C (1 ) Μ : C] 2 ( trc) A 5( C A AC) (6) 10[ Α (1 )( L Μ : Α) ]: C) C D D 2 2 b1 I b2 A b3 A b4 b5 2 (7) In the above equations, A is the secondorder orientation tensor, A fourthorder orientation tensor, C rotary diffusion tensor, W vorticity tensor, D rateofdeformation tensor. Also, L, M are fourthorder tensors, RSC factor, particle shape parameter, and b 1, b 2, b 3, b 4, b 5 are constants for anisotropic rotary diffusion. The fiber length distribution is calculated using a fiberbreakage model as in [4]. In this study, fiber migration or curvature of the fiber is not considered. Mechanical Properties Calculation When fibers are fully aligned and have the uniform length, the stiffness of the composite is calculated as [5] / m f f m : f (8) or / 1 f m f f :: 1 f f (9) 5
6 where f, l, and d are the fiber volume fraction, length, and diameter, respectively., m, and f are the stiffness tensors of the unidirectional (UD) composite, matrix, and fiber, respectively. f is the fiber strainconcentration tensor, and is computed with a selected micromechanical model. The Eshelby MoriTanaka approach [6, 7] gives: f :1 f f (10) with : : f m (11) where S is the Eshelby tensor and I is the fourthorder identity tensor. Due to the fiber breakage during the process, the fiber length is not uniform and the distribution can be described with the probability density function P(l). The stiffness of the composite is: /d d (12) The stiffness tensor / must be calculated for each length segment l i, which requires a lot of computation. To simplify the computation, the average fiber length by weight,, is used in Equation (8) or (9) to calculate the stiffness, i.e. / (13) Then the averaging technique [8] is employed to calculate the composite stiffness averaged over the fiber orientation distribution. The imperfect fiber/matrix interface model by Qu [9] is employed for the expression of the stiffness tensor for a unidirectional composite that contains partially debonded fiber/matrix interfaces. The EshelbyMoriTanaka formulation (9) for the unidirectional composite is modified as: / 1 f m f f :: 1 f f f : f : (14) where the fourthorder tensor is determined from Equation (11) in terms of the modified Eshelby tensor S * given as: 6
7 :: m : (15) in which the fourthorder tensor N is given by (16) where r is the radius of the fiber. represents the compliance in the tangential direction of the interface, and can be expressed in terms of the matrix elastic modulus as. β = 0 corresponds to a perfect fiber/matrix interface while a very high value of represents complete debonding. Components of the fourthorder tensors P and Q for ellipsoidal inclusion are provided by Qu [9]. An Example Case In the example, the software investigated in this report is used to simulate the molding of a panel made of a thermoset material. Figure 2 shows the geometry of the part. Figure 3 shows the simulation model for the initial charge and the part. In this figure, the green area is the final shape of the part to be molded, and the gray area is the initial charge. The length of the part is about 800 mm, the width is 200 mm and the typical thickness of the final part is about 4 mm. The finiteelement mesh has approximately 1,585,000 tetrahedral elements and 276,000 nodes. Figure 2: A geometry model for the part used in the current study. 7
8 Figure 3: A simulation model which shows the part (green) and the initial charge (gray) The following process conditions are used in this example. The initial melt temperature is 45 C, and the mold temperature is 149 C. The nominal fill time is about 12 second. The maximum press force (compression tonnage) is 300 tons and press compression time is 20 seconds. The compression is switched to force control when 99% of the cavity is filled. After that, the press force is maintained at the switchover value for 10 seconds. The press open distance is 27 mm. The press moves at a controlled speed until switch over to force control. The initial press speed is at 3.5 mm/sec, but it drops with time as shown in Figure 4(a). Figure 4(b) shows press displacement versus time. After switch over to force control, the press moves at a constant press force. The total filling and postfilling time is about 40 seconds. The polymer used is a sheet molding compound (SMC) from Premix (PremiGlas 1286). This is a composite material with 34% glass fiber by weight (with initial fiber length of 12 mm). (a) 8
9 (b) Figure 4: (a) Press speed versus time and (b) press displacement versus time. The simulation results and comparison with experiment are shown in Figures Figure 5 shows the pressure distribution in the cavity at two different times during filling. As the initial charge lies near the center of the cavity, the pressure is highest near the center of the cavity. Figure 6 shows the degree of cure distribution near the end of molding. Figure 7 and Figure 8 show the short shot images from the actual molding experiment and simulation. Figure 7 is at time of 5.6 seconds during filling, and Figure 8 is at time of 8.3 second during filling. For Figure 7, the material inside the circular areas at the left and right ends of the part has been removed from the experimental short shots (and so is not shown in the experimental image). Although there are some differences between simulation and experiment, overall, the agreement is reasonable. The difference could be due to the initial charge placement. Since the initial charge is cut and placed in the mold manually, the shape and location of the initial charge can be somewhat different from those used in the simulation. The other potential causes of difference include the effects of fiber orientation on flow (which is neglected in the current study). Figure 9 is the CT (Computed Tomography) scan images of the part which show the fiber orientation. Figure 9 (a) and (b) are images at different layers. Figure 10 shows the fiber orientation (first principal value) obtained from simulation. In this plot, the direction of the long bar represents the direction of the first principal value of orientation. If the value is high (close to 1), it means that more of the fibers are aligned in the first principal direction. Comparison between Figure 9 9
10 and 10 indicate that there are some correlations between the fiber orientation obtained from the experiment and that predicted by the simulation. Figure 11 shows the calculated tensile modulus in the first principal direction. Figure 12 is the calculated Poisson s ratio. Tensile testing experiment was conducted to measure the tensile modulus of the samples produced from the compression molding. Figure 13(a) shows the molded samples which were used to get the specimen, and Figure 13(b) shows the specimen which were cut from the molded sample. The specimen were cut in the length direction and in the transverse (width) direction. Figure 14 shows the comparison of tensile modules obtained from experiment and simulation. The simulation value in this figure is the average tensile modulus value among the nodes within the specimen location. The values measured in X and Y directions are compared. In Figure 14, EX represent the tensile modules value obtained from specimen cut in X direction, and EY in Y direction. X is in the length direction, and Y is in the width direction. As can be seen from this figure, the simulation and experiment values show similar trends although there are some differences in values. (a) (b) Figure 5: Pressure distribution in the cavity during filling at 5.9 second (a) and 13.3 second (b) (in MPa). 10
11 Figure 6: Degree of cure distribution in the part at the end of molding. (a) (b) Figure 7: Short shots from experiment (a) and simulation (b) at 5.6 seconds during filling. 11
12 (a) (b) Figure 8: Short shots from experiment (a) and simulation (b) at 8.3 seconds during filling. 12
13 (a) (b) Figure 9: CT scan images that show the fiber orientation near the right end. Figures (a) and (b) are at different layers. (a) 13
14 (b) Figure 10: Calculated fiber orientation results (first principal value); (a) magnified view near the right end and (b) overall view. Figure 11: Calculated tensile modulus in the first principal direction (in MPa). Figure 12: Calculated Poisson s ratio ( 12 ). 14
15 (a) (b) Figure 13: Samples used in the mechanical property testing: (a) the molded parts where the testing specimen were cut, (b) testing specimen. 15
16 Figure 14: Comparison of tensile modulus values from simulation and experiment in length (X) and width (Y) direction (modulus value in MPa). Conclusion The results from the simulation program developed in this study show that the simulation results for filling pattern, fiber orientation and tensile modulus match reasonably well with the experiment. Acknowledgements We would like to acknowledge the help of Roy Bendickson of Premix Inc. for providing the experimental data used in this report. References 1. S. Han, F. Costa, P. Cook, S. Ray, Threedimensional Simulation of Thermoset Molding Applied to Semiconductorchip Encapsulation, SPE ANTEC, M. R. Kamal and M. E. Ryan, Chapter 4 of Injection and Compression Molding Fundamentals, A. I. Isayev (editor), Marcel Dekker, New York (1987). 16
17 3. J. Wang and X. Jin, Comparison of Recent Fiber Orientation Models in Autodesk Moldflow Insight Simulations with Measured Fiber Orientation Data, Polymer Processing Society 26 th Annual Meeting, X. Jin and J. Wang, Fiber length Distribution Calculation in Injection Molding Simulation, SPE ANTEC, R. Hill, Elastic properties of reinforced solids: Some theoretical principles, Journal of the Mechanics and Physics of Solids, vol. 11, no. 5, pp , Sep J. D. Eshelby, The Determination of the Elastic Field of an Ellipsoidal Inclusion, and Related Problems, Proceedings of the Royal Society A: Mathematical, Physical and Engineering Sciences, vol. 241, no. 1226, pp , Aug T. Mori and K. Tanaka, Average stress in matrix and average elastic energy of materials with misfitting inclusions, Acta Metallurgica, vol. 21, no. 5, pp , May S. G. Advani and C. L. Tucker III, The Use of Tensors to Describe and Predict Fiber Orientation in Short Fiber Composites, Journal of Rheology, vol. 31, no. 8, pp , J. Qu, The effect of slightly weakened interfaces on the overall elastic properties of composite materials, Mechanics of Materials, vol. 14, no. 4, pp , Mar Autodesk and Moldflow are registered trademarks or trademarks of Autodesk, Inc., and/or its subsidiaries and/or affiliates in the USA and/or other countries. All other brand names, product names, or trademarks belong to their respective holders. Autodesk reserves the right to alter product and services offerings, and specifications and pricing at any time without notice, and is not responsible for typographical or graphical errors that may appear in this document Autodesk, Inc. All rights reserved. 17
PROPERTY CALCULATION SYSTEM FOR INJECTION MOLDING AND COMPRESSION MOLDING OF FIBERFILLED POLYMER COMPOSITES
PROPERTY CALCULATION SYSTEM FOR INJECTION MOLDING AND COMPRESSION MOLDING OF FIBERFILLED POLYMER COMPOSITES X. Jin *, J. Wang, S. Han Autodesk Inc., 353 N. Triphammer Rd., Ithaca, NY, 485, U.S.A. Corning
More informationModule 7: Micromechanics Lecture 34: Self Consistent, Mori Tanaka and Halpin Tsai Models. Introduction. The Lecture Contains. Self Consistent Method
Introduction In this lecture we will introduce some more micromechanical methods to predict the effective properties of the composite. Here we will introduce expressions for the effective properties without
More informationAuthors: Correspondence: ABSTRACT:
MultiScale Modeling of the Impact and Failure of Fiber Reinforced Polymer Structures using DIGIMAT to LSDYNA Interface Authors: L. Adam, R. Assaker & R. Ramaya exstream engineering S.A. 7, Rue du Bosquet.
More informationStichwortverzeichnis. Peter Kennedy, Rong Zheng. Flow Analysis of Injection Molds. ISBN (Buch): ISBN (EBook):
Stichwortverzeichnis Peter Kennedy, Rong Zheng Flow Analysis of Injection Molds ISBN (Buch): 9781569905128 ISBN (EBook): 9781569905227 For further information and order see http://www.hanserfachbuch.de/9781569905128
More informationMODELLING THE MECHANICAL AND THERMAL PROPERTIES OF SHORT FIBRE COMPOSITES
MODELLING THE MECHANICAL AND THERMAL PROPERTIES OF SHORT FIBRE COMPOSITES F.W.J. van Hattum 1, C.A. Bernardo 1, F.J. Macedo 2, and J.A. Ferreira 2 1 Department of Polymer Engineering, University of Minho,
More informationFROM PROCESS MODELING TO ELASTIC PROPERTY PREDICTION FOR LONGFIBER INJECTIONMOLDED THERMOPLASTICS 1
FROM PROCESS MODELING TO ELASTIC PROPERTY PREDICTION FOR LONGFIBER INJECTIONMOLDED THERMOPLASTICS 1 Ba Nghiep Nguyen 2 (a), Vlastimil Kunc (b), Barbara J. Frame (b), Jay H. Phelps (c), Charles L. Tucker
More informationThe Significance of the Production Process of FRP Parts for the Performance in Crashworthiness
14 th International LSDYNA Users Conference Session: Simulation The Significance of the Production Process of FRP Parts for the Performance in Crashworthiness Christian Liebold, Andrea Erhart, André Haufe
More informationMicromechanical analysis of FRP hybrid composite lamina for inplane transverse loading
Indian Journal of Engineering & Materials Sciences Vol. 15, October 2008, pp. 382390 Micromechanical analysis of FRP hybrid composite lamina for inplane transverse loading K Sivaji Babu a *, K Mohana
More informationMICROSTRUCTURAL AND ELASTIC PROPERTIES OF SHORT FIBER REINFORCED COMPOSITES
MICROTRUCTURAL AND ELATIC PROPERTIE OF HORT FIBER REINFORCED COMPOITE V. Müller 1, T. Böhlke 1 1 Institute of Engineering Mechanics, Chair for Continuum Mechanics, Karlsruhe Institute of Technology (KIT)
More informationTABLE OF CONTENTS. Mechanics of Composite Materials, Second Edition Autar K Kaw University of South Florida, Tampa, USA
Mechanics of Composite Materials, Second Edition Autar K Kaw University of South Florida, Tampa, USA TABLE OF CONTENTS 1. INTRODUCTION TO COMPOSITE MATERIALS 1.1 Introduction... 1.2 Classification... 1.2.1
More informationMICROMECHANICAL ANALYSIS OF FRP COMPOSITES SUBJECTED TO LONGITUDINAL LOADING
MICROMECHANICAL ANALYSIS OF FRP COMPOSITES SUBJECTED TO LONGITUDINAL LOADING N. Krishna Vihari 1, P. Phani Prasanthi 1, V. Bala Krishna Murthy 2* and A. Srihari Prasad 3 1 Mech. Engg. Dept., P. V. P. Siddhartha
More informationAutodesk Moldflow Insight AMI Fiber Orientation Analysis
Autodesk Moldflow Insight 2012 AMI Fiber Orientation Analysis Revision 1, 22 March 2012. This document contains Autodesk and thirdparty software license agreements/notices and/or additional terms and
More informationSCREW SWIRLING EFFECTS ON FIBER ORIENTATION DISTRIBUTION IN LARGESCALE POLYMER COMPOSITE ADDITIVE MANUFACTURING. Zhaogui Wang*, Douglas E.
Solid Freeform Fabrication 2018: Proceedings of the 29th Annual International Solid Freeform Fabrication Symposium An Additive Manufacturing Conference SCREW SWIRLING EFFECTS ON FIBER ORIENTATION DISTRIBUTION
More informationAnisotropic modeling of short fibers reinforced thermoplastics materials with LSDYNA
Anisotropic modeling of short fibers reinforced thermoplastics materials with LSDYNA Alexandre Hatt 1 1 Faurecia Automotive Seating, Simplified Limited Liability Company 1 Abstract / Summary Polymer thermoplastics
More informationDon Robbins, Andrew Morrison, Rick Dalgarno Autodesk, Inc., Laramie, Wyoming. Abstract
PROGRESSIVE FAILURE SIMULATION OF ASMANUFACTURED SHORT FIBER FILLED INJECTION MOLDED PARTS: VALIDATION FOR COMPLEX GEOMETRIES AND COMBINED LOAD CONDITIONS Don Robbins, Andrew Morrison, Rick Dalgarno Autodesk,
More informationISO 178 INTERNATIONAL STANDARD. Plastics Determination of flexural properties. Plastiques Détermination des propriétés en flexion
INTERNATIONAL STANDARD ISO 178 Fourth edition 20011215 Plastics Determination of flexural properties Plastiques Détermination des propriétés en flexion Reference number ISO 2001 PDF disclaimer This PDF
More informationABSTRACT. Keywords: Birefringence, injection molding, simulation, plastic, viscoelasticity, residual stress, prediction, finite element
Prediction of Birefringence in Plastic Moldings Alexander Bakharev*, Chris Friedl, Franco S. Costa and Peter K. Kennedy Moldflow, 259261 Colchester Rd Kilsyth, Victoria 3137 Australia ABSTRACT This article
More informationMoldflow Report Beaumont Logo. Performed by: Beaumont Technologies Requested by: Customer
Moldflow Report Beaumont Logo Performed by: Beaumont Technologies Requested by: Customer Objective To analyze the BTI Logo part in order to determine an optimal gate location. To thoroughly evaluate the
More informationExperimental Study of the Induced Residual Stresses During the Manufacturing Process of an Aeronautic Composite Material
Research Journal of Applied Sciences, Engineering and Technology 2(6): 596602, 2010 ISSN: 20407467 Maxwell Scientific Organization, 2010 Submitted Date: July 28, 2010 Accepted Date: August 27, 2010 Published
More informationMicromechanics modeling for the stiffness and strength properties of glass fibers/cnts/epoxy composites
High Performance Structures and Materials V 279 Micromechanics modeling for the stiffness and strength properties of glass fibers/cnts/epoxy composites M. Kim, F. A. Mirza & J. I. Song School of Mechatronics
More informationModelling the nonlinear shear stressstrain response of glass fibrereinforced composites. Part II: Model development and finite element simulations
Modelling the nonlinear shear stressstrain response of glass fibrereinforced composites. Part II: Model development and finite element simulations W. Van Paepegem *, I. De Baere and J. Degrieck Ghent
More informationCHAPTER 4 MODELING OF MECHANICAL PROPERTIES OF POLYMER COMPOSITES
CHAPTER 4 MODELING OF MECHANICAL PROPERTIES OF POLYMER COMPOSITES 4. Introduction Fillers added to polymer matrices as additives are generally intended for decreasing the cost (by increase in bulk) of
More informationMultiScale Modeling of Crash & Failure of Reinforced Plastics Parts with DIGIMAT to LSDYNA interface
7 th European LSDYNA Conference MultiScale Modeling of Crash & Failure of Reinforced Plastics Parts with DIGIMAT to LSDYNA interface L. Adam, A. Depouhon & R. Assaker exstream engineering S.A.. 7,
More informationEffect of Specimen Dimensions on Flexural Modulus in a 3Point Bending Test
Effect of Specimen Dimensions on Flexural Modulus in a 3Point Bending Test M. Praveen Kumar 1 and V. Balakrishna Murthy 2* 1 Mechanical Engineering Department, P.V.P. Siddhartha Institute of Technology,
More informationDRAPING SIMULATION. Recent achievements and future trends. Dr. Sylvain Bel LGCIE University Lyon 1
DRAPING SIMULATION Recent achievements and future trends 1 Dr. Sylvain Bel LGCIE University Lyon 1 2 DRAPING SIMULATION Why? How? What? DRAPING SIMULATION WHY? Clamps Punch Fabric Die 1 2 Resin 3 4 Fig.
More informationAPPLICATIONS OF THERMAL ANALYSIS IN POLYMER AND COMPOSITES CHARACTERIZATION. Wei Xie TA Instruments
APPLICATIONS OF THERMAL ANALYSIS IN POLYMER AND COMPOSITES CHARACTERIZATION Wei Xie TA Instruments Abstract Thermal Analysis is the generic name for a series of measurement techniques traditionally used
More informationCLOSED SIMULATION PROCESS CHAIN FOR SHORT FIBER REINFORCED PLASTIC COMPONENTS WITH LSDYNA
CLOSED SIMULATION PROCESS CHAIN FOR SHORT FIBER REINFORCED PLASTIC COMPONENTS WITH LSDYNA B. Lauterbach 1, M. Erzgräber 1, C. Liebold 2, M. Helbig 2, A. Haufe 2 1 Adam Opel AG 2 DYNAmore GmbH www.opel.com
More informationMaterial Testing Overview (THERMOPLASTICS)
Material Testing Overview (THERMOPLASTICS) Table of Contents Thermal Conductivity... 3 Specific Heat... 4 Transition Temperature and Ejection Temperature... 5 Shear Viscosity... 7 PressureVolumeTemperature
More informationModelling the Rheology of SemiConcentrated Polymeric Composites
THALES Project No 1188 Modelling the Rheology of SemiConcentrated Polymeric Composites Research Team Evan Mitsoulis (PI), Professor, NTUA, Greece Costas Papoulias (Research Student), NTUA, Greece Souzanna
More informationComputational Analysis for Composites
Computational Analysis for Composites Professor Johann Sienz and Dr. Tony Murmu Swansea University July, 011 The topics covered include: OUTLINE Overview of composites and their applications Micromechanics
More informationMultiscale analyses of the behaviour and damage of composite materials
Multiscale analyses of the behaviour and damage of composite materials Presented by Didier BAPTISTE ENSAM, LIM, UMR CNRS 8006 151 boulevard de l hôpital l 75013 PARIS, France Research works from: K.Derrien,
More informationHygrothermal stresses in laminates
Hygrothermal stresses in laminates Changing environment conditions (temperature and moisture) have an important effect on the properties which are matrix dominated. Change in temperaturet and moisture
More informationQUESTION BANK Composite Materials
QUESTION BANK Composite Materials 1. Define composite material. 2. What is the need for composite material? 3. Mention important characterits of composite material 4. Give examples for fiber material 5.
More informationME 7502 Lecture 2 Effective Properties of Particulate and Unidirectional Composites
ME 75 Lecture Effective Properties of Particulate and Unidirectional Composites Concepts from Elasticit Theor Statistical Homogeneit, Representative Volume Element, Composite Material Effective Stress
More informationPredicting Elastic Properties of Unidirectional SU8/ZnO Nanocomposites using COMSOL Multiphysics
Predicting Elastic Properties of Unidirectional SU8/ZnO Nanocomposites using COMSOL Multiphysics Neelam Mishra 1, and Kaushik Das *1 1 School of Minerals Metallurgical and Materials Engineering, Indian
More informationTHE MATRIX: EVOLUTIONS II
THE MATRIX: EVOLUTIONS II Pearl Sullivan Composites and Adhesives Group Department of Mechanical Engineering University of Waterloo IPR 28 th Annual Symposium, 16 May 2006 Scope: Multiscale Analyses Atomic/Nanoscale
More informationResidual stresses in short fibre reinforced injection moulded plates
Residual stresses in short fibre reinforced injection moulded plates J. H. D. Voerman August 1996 WB  OK  39 I University of Twente Department of Mechanical Engineering Chair of Design in Plastics Residual
More informationMechanical Engineering Ph.D. Preliminary Qualifying Examination Solid Mechanics February 25, 2002
student personal identification (ID) number on each sheet. Do not write your name on any sheet. #1. A homogeneous, isotropic, linear elastic bar has rectangular cross sectional area A, modulus of elasticity
More informationCOMPUTING MECHANICAL PROPERTIES FROM ORIENTATION TENSORS FOR FIBER FILLED POLYMERS IN AXISYMMETRIC FLOW AND PLANAR DEPOSITION FLOW
COMPUTING MECHANICAL PROPERTIES FROM ORIENTATION TENSORS FOR FIBER FILLED POLYMERS IN AXISYMMETRIC FLOW AND PLANAR DEPOSITION FLOW Blake P. Heller, Douglas E. Smith, David A. Jack Department of Mechanical
More informationModule 7: Micromechanics Lecture 29: Background of Concentric Cylinder Assemblage Model. Introduction. The Lecture Contains
Introduction In this lecture we are going to introduce a new micromechanics model to determine the fibrous composite effective properties in terms of properties of its individual phases. In this model
More informationHOMOGENIZATION OF TRABECULAR BONE MICROSTRUCTURE BASED ON FINITE ELEMENT METHOD AND MICRO COMPUTED TOMOGRAPHY
11th World Congress on Computational Mechanics (WCCM XI) 5th European Conference on Computational Mechanics (ECCM V) 6th European Conference on Computational Fluid Dynamics (ECFD VI) E. Oñate, J. Oliver
More informationBIAXIAL STRENGTH INVESTIGATION OF CFRP COMPOSITE LAMINATES BY USING CRUCIFORM SPECIMENS
BIAXIAL STRENGTH INVESTIGATION OF CFRP COMPOSITE LAMINATES BY USING CRUCIFORM SPECIMENS H. Kumazawa and T. Takatoya Airframes and Structures Group, Japan Aerospace Exploration Agency 6131, Ohsawa, Mitaka,
More information3dimensional joint torque calculation of compression sportswear using 3DCG human model
3dimensional joint torque calculation of compression sportswear using 3DCG human model Akihiro Matsuda, University of Tsukuba Hirokazu Tanaka, University of Tsukuba Hitoshi Aoki, University of Tsukuba
More informationLong glass fiber orientation in thermoplastic composites using a model that accounts for the flexibility of the fibers
Long glass fiber orientation in thermoplastic composites using a model that accounts for the flexibility of the fibers Ortman, K.C. 1, G.M. Vélez 2, A.P.R. Eberle 1, D.G. Baird 1 and P. Wapperom 3 Chemical
More informationAbstract. Introduction
Transient Rheology of a Polypropylene Melt Reinforced with Long Glass Fibers Ortman, K.C. 1, Neeraj Agarwal 1, D.G. Baird 1 and P. Wapperom 2, Jeffrey Giacomin 3 Chemical Engineering Department 1, Virginia
More informationMODELLING THE THERMOELASTIC PROPERTIES OF SHORT FIBRE COMPOSITES WITH ANISOTROPIC PHASES
MODELLING THE THERMOELASTIC PROPERTIES OF SHORT FIBRE COMPOSITES WITH ANISOTROPIC PHASES P.J.Hine*, C.D.Price*, B.Whiteside $, A.M.Cunha # and I.M.Ward* *  IRC in Polymer Science and Technology, University
More informationIdentification of interface properties using Fibre Bragg Grating sensors in a fibre pullout test Gabriel Dunkel, Laurent Humbert and John Botsis
Identification of interface properties using Fibre Bragg Grating sensors in a fibre pullout test Gabriel Dunkel, Laurent Humbert and John Botsis Laboratory of Applied Mechanics and Reliability Analysis
More informationISO 178 INTERNATIONAL STANDARD. Plastics Determination of flexural properties. Plastiques Détermination des propriétés en flexion
INTERNATIONAL STANDARD ISO 178 Fifth edition 20101215 Plastics Determination of flexural properties Plastiques Détermination des propriétés en flexion Reference number ISO 178:2010(E) ISO 2010 PDF disclaimer
More informationEVALUATION OF GLASS FIBER/EPOXY INTERFACIAL STRENGTH USING A CRUCIFORM SPECIMEN
6 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS EVALUATION OF GLASS FIBER/EPOXY INTERFACIAL STRENGTH USING A CRUCIFORM SPECIMEN Shinji Ogihara*, Yoriaki Sakamoto ** and Hajime Kato ** *Department
More informationStiffness Predictions for Unidirectional ShortFiber Composites: Review and Evaluation
Stiffness Predictions for Unidirectional ShortFiber Composites: Review and Evaluation Charles L. Tucker III Department of Mechanical and Industrial Engineering University of Illinois at UrbanaChampaign
More informationHysteretic equivalent continuum model of nanocomposites with interfacial stickslip
Hysteretic equivalent continuum model of nanocomposites with interfacial stickslip Giovanni Formica 1, Michela Talò, Walter Lacarbonara 1 Dipartimento di Architettura, Università degli Studi Roma Tre
More informationRELATIONSHIP BETWEEN RADIAL COMPRESSIVE MODULUS OF ELASTICITY AND SHEAR MODULUS OF WOOD Jen Y. Liu Research Engineer
RELATIONSHIP BETWEEN RADIAL COMPRESSIVE MODULUS OF ELASTICITY AND SHEAR MODULUS OF WOOD Jen Y. Liu Research Engineer and Robert J. Ross Supervisory Research Engineer USDA Forest Service Forest Products
More informationSize Effect of Clay Filler Particles on Mechanical Properties of Pultruded Polymer Composites Under Shear Loading
Minnesota State University, Mankato Cornerstone: A Collection of Scholarly and Creative Works for Minnesota State University, Mankato All Theses, Dissertations, and Other Capstone Projects Theses, Dissertations,
More informationAspect Ratio Requirements for NanotubeReinforced, PolymerMatrix Composites
Aspect Ratio Requirements for NanotubeReinforced, PolymerMatrix Composites J.A.Nairn Wood Science and Engineering, Oregon State University, Corvallis, OR 97330, USA Abstract A fiber s efficiency in a
More informationSoufiane Belhouideg. Keywords Composite materials, homogenization method, Eshelby s inclusion problem.
Prediction of effective mechanical properties of composite materials using homogenization approach: Application to tungsten fiber reinforced bulk metallic glass matrix composite Soufiane Belhouideg Abstract
More informationKINK BAND FORMATION OF FIBER REINFORCED POLYMER (FRP)
KINK BAND FORMATION OF FIBER REINFORCED POLYMER (FRP) 1 University of Science & Technology Beijing, China, niukm@ustb.edu.cn 2 Tsinghua University, Department of Engineering Mechanics, Beijing, China,
More informationME 582 Advanced Materials Science. Chapter 2 Macromechanical Analysis of a Lamina (Part 2)
ME 582 Advanced Materials Science Chapter 2 Macromechanical Analysis of a Lamina (Part 2) Laboratory for Composite Materials Research Department of Mechanical Engineering University of South Alabama, Mobile,
More informationINTERNATIONAL JOURNAL OF APPLIED ENGINEERING RESEARCH, DINDIGUL Volume 2, No 1, 2011
Interlaminar failure analysis of FRP cross ply laminate with elliptical cutout Venkateswara Rao.S 1, Sd. Abdul Kalam 1, Srilakshmi.S 1, Bala Krishna Murthy.V 2 1 Mechanical Engineering Department, P. V.
More informationPart 7. Nonlinearity
Part 7 Nonlinearity Linear System Superposition, Convolution re ( ) re ( ) = r 1 1 = r re ( 1 + e) = r1 + r e excitation r = r() e response In the time domain: t rt () = et () ht () = e( τ) ht ( τ) dτ
More informationModule III  Macromechanics of Lamina. Lecture 23. MacroMechanics of Lamina
Module III  Macromechanics of Lamina Lecture 23 MacroMechanics of Lamina For better understanding of the macromechanics of lamina, the knowledge of the material properties in essential. Therefore, the
More informationUniversity of Sheffield The development of finite elements for 3D structural analysis in fire
The development of finite elements for 3D structural analysis in fire Chaoming Yu, I. W. Burgess, Z. Huang, R. J. Plank Department of Civil and Structural Engineering StiFF 05/09/2006 3D composite structures
More informationModule 4: Behaviour of a LaminaeII. Learning Unit 1: M1. M4.1 Mechanics of Composites. M4.1.1 Introduction to Mechanics of Composites
Module 4: Behaviour of a LaminaeII Learning Unit 1: M1 M4.1 Mechanics of Composites M4.1.1 Introduction to Mechanics of Composites The relation between ply uniaxial strengths and constituent properties
More informationDigimat material model for short fiber reinforced plastics at Volvo Car Corporation
Digimat material model for short fiber reinforced plastics at Volvo Car Corporation Mats Landervik DYNAmore Nordic Johan Jergeus Volvo Car Corporation June 2, 2015 26TH SICOMP CONFERENCE, GOTHENBURG 1
More informationMechanical and Thermal Properties of Coir Fiber Reinforced Epoxy Composites Using a Micromechanical Approach
Mechanical and Thermal Properties of Coir Fiber Reinforced Epoxy Composites Using a Micromechanical Approach Sandhyarani Biswas Department of Mechanical Engineering, N.I.T Rourkela, INDIA Abstract: Nowadays,
More informationThe University of Melbourne Engineering Mechanics
The University of Melbourne 436291 Engineering Mechanics Tutorial Four Poisson s Ratio and Axial Loading Part A (Introductory) 1. (Problem 922 from Hibbeler  Statics and Mechanics of Materials) A short
More informationTHE INFLUENCE OF INPLANE DENSITY VARIATION ON ENGINEERING PROPERTIES OF ORIENTED STRANDBOARD: A FINITE ELEMENT SIMULATION
Proceedings of McMat5: 5 Joint ASME/ASCE/SES Conference on Mechanics and Materials June 13, 5, Baton Rouge, Louisiana, USA 255 THE INFLUENCE OF INPLANE DENSITY VARIATION ON ENGINEERING PROPERTIES OF
More informationModeling the Rheology and Orientation Distribution of Short Glass Fibers Suspended in Polymeric Fluids: Simple Shear Flow
Modeling the Rheology and Orientation Distribution of Short Glass Fibers Suspended in Polymeric Fluids: Simple Shear Flow Aaron P.R. berle, Donald G. Baird, and Peter Wapperom* Departments of Chemical
More informationINTERFACIAL STRENGTH EVALUATION IN A GLASS FIBER REINFORCED COMPOSITE USING CRUCIFORM SPECIMEN METHOD
INTERFACIAL STRENGTH EVALUATION IN A GLASS FIBER REINFORCED COMPOSITE USING CRUCIFORM SPECIMEN METHOD Shinji Ogihara, oriaki Sakamoto 2, Hajime Kato 2, Satoshi Kobayashi 3 and Ichiro Ueno Dept. of Mechanical
More informationPrediction of Elastic Constants on 3D Fourdirectional Braided
Prediction of Elastic Constants on 3D Fourdirectional Braided Composites Prediction of Elastic Constants on 3D Fourdirectional Braided Composites Liang Dao Zhou 1,2,* and Zhuo Zhuang 1 1 School of Aerospace,
More informationModelling of viscoelastic properties of a curing adhesive
Computational Methods and Experiments in Materials Characterisation III 241 Modelling of viscoelastic properties of a curing adhesive J. de Vreugd 1, K. M. B. Jansen 1, L. J. Ernst 1 & J. A. C. M. Pijnenburg
More informationChapter 2: Elasticity
OHP 1 Mechanical Properties of Materials Chapter 2: lasticity Prof. Wenjea J. Tseng ( 曾文甲 ) Department of Materials ngineering National Chung Hsing University wenjea@dragon.nchu.edu.tw Reference: W.F.
More informationMulti Disciplinary Delamination Studies In Frp Composites Using 3d Finite Element Analysis Mohan Rentala
Multi Disciplinary Delamination Studies In Frp Composites Using 3d Finite Element Analysis Mohan Rentala Abstract: FRP laminated composites have been extensively used in Aerospace and allied industries
More informationTHE TRANSVERSE OFFAXIS STIFFNESS AND STRENGTH OF SOFTWOODS. Abstract
THE TRANSVERSE OFFAXIS STIFFNESS AND STRENGTH OF SOFTWOODS Carl S. Moden 1, Jessica Polycarpe 1 and Lars A. Berglund 2 1 Dept. of Aeronautical and Vehicle Engineering The Royal Institute of Technology
More informationIJSER 1. INTRODUCTION. M.Elhadary
1591 A new failure criterion for GRP composite materials subjected to inphase and outofphase biaxial fatigue loading under different stress ratios M.Elhadary Abstract this studying the fatigue behavior
More informationDAMAGE SIMULATION OF CFRP LAMINATES UNDER HIGH VELOCITY PROJECTILE IMPACT
18 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS DAMAGE SIMULATION OF CFRP LAMINATES UNDER HIGH VELOCITY PROJECTILE IMPACT A. Yoshimura 1*, T. Okabe, M. Yamada 3, T. Ogasawara 1, Y. Tanabe 3 1 Advanced
More informationA Constitutive Framework for the Numerical Analysis of Organic Soils and Directionally Dependent Materials
Dublin, October 2010 A Constitutive Framework for the Numerical Analysis of Organic Soils and Directionally Dependent Materials FracMan Technology Group Dr Mark Cottrell Presentation Outline Some Physical
More informationThe effect of melt compressibility on the mold filling of thinwalled parts
The effect of melt compressibility on the mold filling of thinwalled parts Andy Rose, Lucien Douven, DSM Ahead BV Autodesk Moldfow, Benelux user meeting Eindhoven May 2 nd, 2017 Agenda Introduction Background
More informationSTEEL FIBER CURVATURE IN CONCRETE COMPOSITES: MODULUS PREDICTIONS USING EFFECTIVE STEEL FIBER PROPERTIES
American Journal of Applied Sciences 11 (1): 145151, 2014 ISSN: 15469239 2014 Science Publication doi:10.3844/ajassp.2014.145.151 Published Online 11 (1) 2014 (http://www.thescipub.com/ajas.toc) STEEL
More informationExercise: concepts from chapter 8
Reading: Fundamentals of Structural Geology, Ch 8 1) The following exercises explore elementary concepts associated with a linear elastic material that is isotropic and homogeneous with respect to elastic
More informationPolymer engineering syllabus (BSc)
Polymer engineering syllabus (BSc) First semester Math 1 Physics 1 Physics 1 lab General chemistry General chemistry lab workshop Second semester Math 2 Physics 2 Organic chemistry 1 Organic chemistry
More informationMultimode revisited
Multimode revisited Testing the application of shift factors S.J.M Hellenbrand 515217 MT 7.29 Coaches: Ir. L.C.A. van Breemen Dr. Ir. L.E. Govaert 27 7 Contents Contents 1 Introduction 2 I Polymers
More informationUNIVERSITY OF SASKATCHEWAN ME MECHANICS OF MATERIALS I FINAL EXAM DECEMBER 13, 2008 Professor A. Dolovich
UNIVERSITY OF SASKATCHEWAN ME 313.3 MECHANICS OF MATERIALS I FINAL EXAM DECEMBER 13, 2008 Professor A. Dolovich A CLOSED BOOK EXAMINATION TIME: 3 HOURS For Marker s Use Only LAST NAME (printed): FIRST
More informationMaterial Testing Report SN 7131 ISOFIL HK 30 TTH0 WT0822
Material Testing Report SN 7131 ISOFIL HK 30 TTH0 WT0822 Prepared for: SIRMAX SPA Via Dell Artigianato 42 Cittadella 35013 Italy Prepared by: Autodesk Moldflow Plastics Labs 2353 N. Triphammer Rd. Ithaca,
More informationMATERIAL MECHANICS, SE2126 COMPUTER LAB 4 MICRO MECHANICS. E E v E E E E E v E E + + = m f f. f f
MATRIAL MCHANICS, S226 COMPUTR LAB 4 MICRO MCHANICS 2 2 2 f m f f m T m f m f f m v v + + = + PART A SPHRICAL PARTICL INCLUSION Consider a solid granular material, a so called particle composite, shown
More informationImproved stress prediction in adhesive bonded optical components
Improved stress prediction in adhesive bonded optical components J. de Vreugd 1a, M.J.A. te Voert a, J.R. Nijenhuis a, J.A.C.M. Pijnenburg a, E. Tabak a a TNO optomechatronics, Stieltjesweg 1, 2628 CK,
More informationWith Autodesk Advanced Material Exchange and Abaqus to precise results of structural FEM for fiber reinforced polymers
With Autodesk Advanced Material Exchange and Abaqus to precise results of structural FEM for fiber reinforced polymers Case study of a comprehensive approach to prove that coupling structural FEM and process
More informationTheory at a Glance (for IES, GATE, PSU)
1. Stress and Strain Theory at a Glance (for IES, GATE, PSU) 1.1 Stress () When a material is subjected to an external force, a resisting force is set up within the component. The internal resistance force
More informationInfluence of fibre proportion and position on the machinability of GFRP composites An FEA model
Indian Journal of Engineering & Materials Sciences Vol. 12, October 2005, pp. 443450 Influence of fibre proportion and position on the machinability of GFRP composites An FEA model D Abdul Budan* Department
More informationChapter 1 Fluid Characteristics
Chapter 1 Fluid Characteristics 1.1 Introduction 1.1.1 Phases Solid increasing increasing spacing and intermolecular liquid latitude of cohesive Fluid gas (vapor) molecular force plasma motion 1.1.2 Fluidity
More informationRelease Notes Digimat 6.0.1
Release Notes Digimat 6.0.1 May 2015 p. 2 p. 3 p.4 p. 6 p. 7 p. 9  p.10 1 P a g e C o p y r i g h t M S C S o f t w a r e B e l g i u m, 2015 New Capabilities Failure indicators o Temperature dependent
More informationSOME RESEARCH ON FINITE ELEMENT ANALYSIS OF COMPOSITE MATERIALS
Mechanical Testing and Diagnosis ISSN 2247 9635, 2012 (II), Volume 3, 7985 SOME RESEARCH ON FINITE ELEMENT ANALYSIS OF COMPOSITE MATERIALS Valeriu DULGHERU, Viorel BOSTAN, Marin GUŢU Technical University
More informationPrediction of Micromechanical Behaviour of Elliptical Frp Composites
Prediction of Micromechanical Behaviour of Elliptical Frp Composites Kiranmayee.Nerusu Dept. of Mechanical Engg. P. V. P. Siddhartha Institute of Technology, Vijayawada 520 007, A.P, India. P. Phani Prasanthi
More informationISSN: ISO 9001:2008 Certified International Journal of Engineering Science and Innovative Technology (IJESIT) Volume 2, Issue 4, July 2013
Delamination Studies in FibreReinforced Polymer Composites K.Kantha Rao, Dr P. Shailesh, K. Vijay Kumar 1 Associate Professor, Narasimha Reddy Engineering College Hyderabad. 2 Professor, St. Peter s Engineering
More informationEffects of geometry and properties of fibre and matrix on overall. composite parameters
Int. Journal of Applied Sciences and ngineering Research, ol. 3, Issue 4, 2014 www.ijaser.com 2014 by the authors Licensee IJASR Under Creative Commons License 3.0 editorial@ijaser.com Research article
More informationME Final Exam. PROBLEM NO. 4 Part A (2 points max.) M (x) y. z (neutral axis) beam crosssec+on. 20 kip ft. 0.2 ft. 10 ft. 0.1 ft.
ME 323  Final Exam Name December 15, 2015 Instructor (circle) PROEM NO. 4 Part A (2 points max.) Krousgrill 11:30AM12:20PM Ghosh 2:303:20PM Gonzalez 12:301:20PM Zhao 4:305:20PM M (x) y 20 kip ft 0.2
More informationMeasurement of the Transverse and Longitudinal Viscosities of Continuous Fibre Reinforced Composites
Measurement of the ransverse and Longitudinal Viscosities of Continuous Fibre Reinforced Composites P. Harrison,. Haylock and A.C. Long University of Nottingham  School of Mechanical, Materials & Manufacturing
More informationFINITE ELEMENT ANALYSIS OF COMPOSITE MATERIALS
FINITE ELEMENT ANALYSIS OF COMPOSITE MATERIALS Ever J. Barbero Department of Mechanical and Aerospace Engineering West Virginia University USA CRC Press Taylor &.Francis Group Boca Raton London New York
More informationInstitut de Recherche en Génie Civil et Mécanique, Ecole Centrale de Nantes, 1, Rue de la Noé, Nantes France
Characterization of an aeronautic composite material during the manufacturing process Experimental study of the process induced residual stresses throughthethickness Youssef Abou Msallem 1, Frédéric
More informationInfluence of residual stresses in the structural behavior of. tubular columns and arches. Nuno Rocha Cima Gomes
October 2014 Influence of residual stresses in the structural behavior of Abstract tubular columns and arches Nuno Rocha Cima Gomes Instituto Superior Técnico, Universidade de Lisboa, Portugal Contact:
More informationComparison of Plywise StressStrain results for graphite/epoxy laminated plate subjected to inplane normal loads using CLT and ANSYS ACP PrepPost
Comparison of Plywise StressStrain results for graphite/epoxy laminated plate subjected to inplane normal loads using CLT and ANSYS ACP PrepPost 1 Mihir A. Mehta, 2 Satyen D. Ramani 1 PG Student, Department
More information